Advances in Physics Theories and Applications ISSN 2224-719X (Paper) ISSN 2225-0638 (Online) Vol.19, 2013 - Selected from International Conference on Recent Trends in Applied Sciences with Engineering Applications

www.iiste.org

Thermoelastic Behaviour of Orientationally Disordered (NH4Br) x (KBr) 1-x Alpana Tiwari* (Corresponding author) Government M.L.B.Girls P.G.College, Bhopal-462002 .India. Phone: +91-0755-2660717, Fax: +91-0755-2661783 E-mail alpanatiwari@gmail.com N. K. Gaur Department of Physics, Barkatullah University, Bhopal – 462026, India Phone: +91-0755-2491821, Fax: +91-0755-2491823 Abstract We have incorporated the translational rotational (TR) coupling effects in the framework of three body force shell model (TSM) to develop an extended TSM (ETSM). This ETSM has been applied to reveal the second order elastic constants (C11,C12 and C44) in the dilute regimes 0≤ x ≤ 0.50 as a function of temperature for 0K≤T≤320K. The anomalous elastic behaviour in C44 has been depicted well by ETSM results in the orientationally disordered (NH4Br) x(KBr)1-x mixed crystals. In order to present a visual comparison of the TRcoupling effect on second order elastic constants, we have evaluated the SOECs with and without TR coupling term in ETSM. Keywords: Orientational glass, TR-coupling, Elastic constants. 1. Introduction In the past few years, an enormous amount of research has been devoted to investigate the static and dynamic behavior of the mixed molecular crystals. These mixed crystals exhibit an orientational glass state at low temperatures. They represent a new class of disordered solids which serve as a conceptual link for an understanding of dynamic processes in glasses [1, 2]. When the tetrahedral NH4+ molecules in ammonium bromide are statistically diluted by spherical K+ ions, the mixed crystals (NH4Br)x(KBr)1-x exhibit an orientational glass state at low temperatures[3]. It is well known that mixed crystals (NH4Br)x(KBr)1-x possess rocksalt (NaCl) structures at room temperature and over certain concentration (x) range. This NaCl phase is characterized by a dynamical disorder of the NH4 molecules. Below the critical concentration xc=0.55, the cubic order of the center of mass lattice is preserved for all the temperatures and a freezing transition of orientational degrees of freedom is found. The neutron scattering experiments and infrared spectroscopy revealed a quasielastic line width indicating the existence of orientational glass (OG) state in (NH4Br) x(KBr)1-x mixed crystals. In the dynamically disordered phase, distortions are introduced due to non-equivalence of N-H bonds, which induce elastic quadrupolar moments of NH4+ions in (NH4Br)x(KBr)1-x mixed systems. Although the average symmetry of these crystals is cubic, but the orientational disorder locally breaks the cubic symmetry and anomalous softening of sheer elastic constant C44 is observed. The reason for the same has been attributed to the coupling of rotator function to long wavelength acoustic displacements, popularly known as the translationalrotational (TR) coupling [3-7]. Singh and Gaur [8] incorporated the effects of TR coupling in the framework of a realistic three body force shell model (TSM) [9] to develop ETSM. It has been applied successfully by Gaur et.al. to explain the elastic, thermal and dynamical properties of the orientationally disordered alkali cyanides, their mixed crystal counterparts, sodium superoxide, ammonium halides and ammonium-alkali halide mixed crystals [10-16]. The present theoretical approach is motivated from the versatility and considerable success of the ETSM. We have applied this ETSM to investigate the temperature dependence of the second order elastic constants of (NH4Br)x(KBr)1-x. The essential formulation of the present model is given in the next section and the results obtained by us are presented and discussed in the subsequent section. 1.1 Formulation of ETSM The interionic interaction potential of ETSM has been expressed as [8] 2 + ' − ' φ = − e ∑Zk Zk' rk−1k' 1+ ∑ f k (rkk') − ∑ckk' rk−k6' − ∑d kk' rk−8k' + b∑β kk' exprk rk rkk + φTR ρ 2 kk' k k' k k' kk'

(1)

Here, k(k’) denote the positive (negative) ions and sum is taken over all the (kk’) ions. In the above expression, the first two terms represent the long-range Coulomb and three body interactions (TBI) [9]. The third and fourth terms are the additional van der Waals (vdW) attraction terms due to the dipole–dipole (d-d) and dipole– quadrupole (d–q) interactions [17]. The fifth term is the Hafemeister and Flygare (HF) type short-range (SR) 1

Advances in Physics Theories and Applications ISSN 2224-719X (Paper) ISSN 2225-0638 (Online) Vol.19, 2013 - Selected from International Conference on Recent Trends in Applied Sciences with Engineering Applications

www.iiste.org

overlap repulsion [18] extended upto the second neighbour ions. βkk’ are the Pauling coefficients. The last term, ΦTR is the new contribution due to the translation-rotational (TR) coupling. The TR coupling coefficients are obtained on the lines of Sahu and Mahanti (19, 20). The expressions for TR coupling coefficients are given a little later. Here, b and ρ are the hardness and range parameters. The TR coupling effects have been introduced through the second order elastic constants (SOECs) derived from the Eq. (1) and expressed as [8]:

Cij = Cij0 + δCijTR

(2)

0

TR

with Cij as their unrenormalized values and Cij are the TR coupling contributions to the SOECs. For the calculation of CijTR, we have used the expressions as given in ref.[21].

8 a

δC11TR = − Aeff2 χ11 (T )

(3)

4 2 Aeff χ 11 (T ) a 2 = − Beff2 χ 44 (T ) a

δC12TR =

(4)

TR δC 44

(5)

Here, a is the lattice constant. The effective coupling constants Aeff and Beff are given by Aeff =AR+AQ and Beff = BR +BQ (6) with AR and BR as the parameters associated with the short-range repulsive interactions and AQ and BQ are associated with the quadrupole electric field gradient interaction given by Michel and Naudts [22] and Sahu and Mahanti [23] as (7) AR = √5π (b/ρ) (d2+a2) -1/2 [a(3f2–f0) +d(f1 –3f3)] BR=-√30π (b/ρ) (d2+a2)-1/2[d (f1–3f3)] With

(8)

1+ g

f 0 = − g ( n +1)

∫ (1 −

y 2 ) n e − yh dy

1− g

(9) Where, h= (1/ρ) (d2+a2)1/2 and g = 2da/ (d2+a2) The various symbols appearing in the above eqns. (3) to (9) are explained in ref. [23]. The quadrupole electric field gradient interaction AQ and BQ and the SR repulsive interaction parameters AR and BR are calculated using their expressions from [23] and the method [10]. The calculated values of these parameters and the vdW coefficients are listed in Table 1. The susceptibility χ11 is related to C11 and C12 through Aeff, while χ44 is related to C44 through Beff. The computed results on the elastic constants (C11, C12, C44) of (NH4Br)x(KBr)1-x.are presented and discussed below. 1.1.1 Results and Discussions The values of the vdW coefficients (Ckk’ and dkk’) and their overall coefficients (C, D) for NH4Br and KBr have been evaluated by us using their expressions reported elsewhere [17]. Their estimated values are listed in Table 1 and used to compute their values for the mixed crystals (NH4Br)x(KBr)1-x applying the Vegard’s law [24]. The model parameters (b,f(r)) have been evaluated from the equilibrium condition and using the input data (ro, B) from Table 2 and the values of vdW and TR-coupling coefficients listed in Table 1. The values of the model parameters thus obtained have also been depicted in Table 2. The values of the first and second order space derivatives of f(r) have been evaluated from the relation [25] f(r) = fo exp (-r/) (10) The novelty in our calculations lies in the fact that we have not used those properties as the input data which are intended for the prediction. In order to obtain such input data at different temperatures, we have used the thermal expansion relation. Also, we have obtained the values of the counterparts mixed crystal at different concentrations (x) by applying the well known Vegard’s law [24]. Experimentally determined values of r0 at various concentrations have been used [5]. Using the expressions given in [12], we have computed the values of the second order elastic constants (C11, C12 and C44) as a function of temperature 0K<T<320K for dilute regimes 0≤x≤0.50. while computing these elastic constants, the contributions from the translational-rotational coupling are taken into account. This TR coupling has played a significant role in explaining the anomalous behaviour of the sheer elastic constant (C44) of the mixed crystals below the temperature, T=60K and x = 0.30, 0.40 and 0.50. The values of the second order elastic constants obtained from ETSM have been plotted as a function of temperature and concentration (x) as displayed in fig.1. For all the concentrations (x=0.10 to 0.50), the values of

2

Advances in Physics Theories and Applications ISSN 2224-719X (Paper) ISSN 2225-0638 (Online) Vol.19, 2013 - Selected from International Conference on Recent Trends in Applied Sciences with Engineering Applications

www.iiste.org

C11 (fig.1a) are decreasing with temperature, while on the contrary values of C12 (fig.1b) are increasing with the increase of temperature and this feature is usual behaviour of the rocksalt structure materials. Also, there is no remarkable change in the values of C11 and C12 for different concentrations (x=0.10 to 0.50). The reason for this decrease of C11 for all the concentrations has been ascribed by Berret et.al. [26] to anharmonic three phonon interaction process. Though experimental observations are not available for these mixed crystals but a similar trend of variation is revealed from the experimentally observed data [26] for ammonium iodide mixed crystals of same class [15].However, the effects of the concentration (x=0.10 to 0.50) on the shear elastic constant (C44) are more pronounced (see fig1c), but weak as compared to those obtained in cyanide halide mixed crystals [27].This suggests that the magnitude of the quadrupole moment of ammonium molecular ion (NH4+) is small and the effect of TR-coupling is weak in (NH4Br)x(KBr)1-x. At lower ammonium concentration (x=0.10, 0.20), the values of C44 remain nearly constant in the temperature range 0K<T<320K. However, an anomalous softening of the shear elastic constant (C44) is noticed (fig. 1c) to occur below 60K for higher concentrations (x = 0.30, 0.40 and 0.50). This anomaly can be attributed to the TR coupling [19, 22, 26] of the quadrupole moments of the NH4+ ions with the sheer modes [26]. It has been observed that the agreement improve quite significantly in all the cases of inclusion of TR coupling denoted by ‘x’.It is noticed in fig.1c when we evaluate C44 with TR coupling, softening is observed at lower temperatures, which is not found in the absence of TR coupling term. Hence it may be concluded that the softening can be seen only by incorporating the TR coupling in the formulation of TSM. This implies that ETSM formalism properly incorporates the TR coupling effects in (NH4Br)x(KBr)1-x. Values of C11, C12 and C44 for which the comparison could not be made due to the lack of experimental data shall work as a guide to the experimental workers in future. It is interesting to note that the anomalous softening occurring in C44 below the intermediate temperature range is similar to the observed variations in mixed crystals of the same class [26]. 1.1.2 Conclusion The present ETSM has been applied to explore the elastic properties of the orientationally disordered ammonium alkali bromide. It can be concluded on the basis of the above discussions that our theoretical results for elastic properties show the similar behaviour as experimentally observed for the orientationally disordered mixed crystals of same category and are reasonably good. This is not unexpected as the ETSM framework is capable to account for the effects of the Cauchy violations (elastic properties), the realistic interaction potential, the polarizibilities (dielectric properties) and the TR coupling effects for the present system of orientationally disordered mixed materials. A detailed description of the theoretical investigation of the second order elastic constants of the orientationally disordered ammonium bromide mixed crystals has been presented in this paper. Here the results on elastic constants are of academic interest at present but it may serve as a guide to the experimental workers in future. References 1. I. Fehst et.al., Phys. Rev. Lett. 64 (1990) 3139. 2. Hochli U.T., Knorr K. and Loidl A., Adv. Phys. 39 (1990) 405. 3. R.Bohmer, F.Fujara and G.Hinze, Sol. State Communications 86 (1993)183. 4. M. Ohl,F.Mayr M.Reehuis,W.Schmidt and A.Loidl, J. Phys. Condensed. Matter 13 (2001)10221. 5. J.F.Berret, J.L.Sauvajol and B. Hennion, J. Phys.Condensed. Matter 4 (1992) 9235. 6. M. Paasch et.al., Z. Phys. B 99 (1996) 333. 7. J.F.Berret, J.L.Sauvajol, B.Hennion, C.Bostoen and S.Haussühl, Europhys. Lett. 16(1) (1991) 91. 8. R.K. Singh and N.K. Gaur, Z. Phys. B75 (1989) 127. 9. R. K. Singh, Phys. Reports 85 (1982) 259. 10. N.K. Gaur, N. Kaur, J. Galgale, M. Manke and R.K. Singh, Mod. Phys. Lett. B 17 (2003) 1391. 11. N.K. Gaur, P. Singh, E.G. Rini, J. Galgale and R.K. Singh, Pramana J. Phys. 63 (2004) 419. 12. P. Singh, N.K. Gaur and R.K. Singh, Phys. Stat. Solidi (b) 244 (2007) 3099. 13. P. Singh and N.K. Gaur, Phys. Lett. A 371(2007) 349. 14. Alpana Tiwari, N. K. Gaur and R.K.Singh, Phys. Stat. Sol.B 246 (2009) 1215. 15. Alpana Tiwari, N. K. Gaur and R.K.Singh, J. Phys. Chem. Solids 71 (2010) 717. 16. Alpana Tiwari, N.K.Gaur and Preeti Singh, J. Phys. Conference series 215 (2010) 012062. 17. M.P. Tosi and F.G. Fumi, J. Phys. Chem. Solids 23 (1962) 356; M.P. Tosi, Sol. State Phys. 2 (1964) 1. 18. D.W. Hafemeister and W.H. Flygare, J. Chem. Phys. 43 (1965) 795. 19. S.D. Mahanti and D. Sahu, Phys. Rev. Lett. 48 (1982) 936. 20. D. Sahu and S.D. Mahanti, Phys. Rev. B (1984) 340. 21. D.Sahu and S.D. Mahanti, Sol. State. Commn. 47 (1983) 207. 22. K.H. Michel and J. Naudts, Phys. Rev. Lett. 39 (1977) 212. 23. D. Sahu and S.D. Mahanti, Phys. Rev. B 26 (1982) 2981.

3

24. 25. 26. 27.

www.iiste.org

Vegards L, Z. Phys., 5 (1921) 17. W. Cochran, CRC Rev. Sol. State Sc. 2 (1971) 1. J.F.Berret et.al., Sol. State Communications 74 (1990) 1041. K.Knorr, Phys. Rev. Lett. 63 (1989) 2749.

Table 1. The van der Waals coefficients (ckk and dkk in the units of 10-60erg/ cm6 and 10−76erg/ cm8, respectively) of NH4Br & KBr and TR coupling parameters for NH4Br at 300K. Values vdW coefficients TR-coupling Parameters Values NH4Br KBr AR (10-4dyn) -0.080 c 181.07 36.40 kk

ckk’

323.71

94.90

BR (10-4dyn) -4

0.798

ck’k’

585.40

266.90

AQ (10 dyn)

0.221

dkk

100.68

54.40

BQ (10-4dyn)

-0.187

dkk’

203.24

197.30

dk'k'

405.02

715.70

C

4177

898

D

2213

1520

Table 2. Model parameters for (NH4Br)x(KBr)1-x at 300K. Concentration x

b (1012erg)

Model Parameters f (r)

0.10

2.966

ρ (Å) 3.535

0.20

3.041

3.675

-0.136

0.30

3.093

3.871

-0.050

0.40

3.120

3.880

0.040

3.128

3.892

0.135

0.50

-0.218

Figure 1. SOECs C11 (a), C12(b) and C44(c) for (NH4Br)x (KBr)1-xfor 0< x < 0.50 and 0< T < 320K. ‘wtr’ represents the curves without TR coupling.

4

7.5

4.5

(a)

(b) 6.5

3.5

C121010dyne/cm 2

4.0

x=0.10 x=0.20 x=0.30 x=0.40 x=0.50 wt r0.10 wt r0.20 wt r0.30 wt r0.40 wt r0.50

3.0

2.5 0

100

T(K)

200

5.5

x=0.10 x=0.20 x=0.30 x=0.40 x=0.50 wtr0.10 wtr0.20 wtr0.30 wtr0.40 wtr0.50

4.5

3.5 0

300

100

T(K)

7.5

(c) 7.0 C441010dyne/cm 2

C111011dyne/cm 2

www.iiste.org

6.5 x=0.10 x=0.20 x=0.30 x=0.40 x=0.50 wt r0.10 wt r0.20 wt r0.30 wt r0.40 wt r0.50

6.0 5.5 5.0 4.5 0

100

T(K)

5

200

300

200

300

This academic article was published by The International Institute for Science, Technology and Education (IISTE). The IISTE is a pioneer in the Open Access Publishing service based in the U.S. and Europe. The aim of the institute is Accelerating Global Knowledge Sharing. More information about the publisher can be found in the IISTEâ€™s homepage: http://www.iiste.org CALL FOR PAPERS The IISTE is currently hosting more than 30 peer-reviewed academic journals and collaborating with academic institutions around the world. Thereâ€™s no deadline for submission. Prospective authors of IISTE journals can find the submission instruction on the following page: http://www.iiste.org/Journals/ The IISTE editorial team promises to the review and publish all the qualified submissions in a fast manner. All the journals articles are available online to the readers all over the world without financial, legal, or technical barriers other than those inseparable from gaining access to the internet itself. Printed version of the journals is also available upon request of readers and authors. IISTE Knowledge Sharing Partners EBSCO, Index Copernicus, Ulrich's Periodicals Directory, JournalTOCS, PKP Open Archives Harvester, Bielefeld Academic Search Engine, Elektronische Zeitschriftenbibliothek EZB, Open J-Gate, OCLC WorldCat, Universe Digtial Library , NewJour, Google Scholar